X‑ray Diﬀraction, Mö ssbauer Spectroscopy, Magnetic Susceptibility, and Speciﬁc Heat Investigations of Na4NpO5 and Na5NpO6 Anna L. Smith,*,†,‡ Amir Hen,† Philippe E. Raison,*,† Eric Colineau,† Jean-Christophe Griveau,† Nicola Magnani,† Jean-Pierre Sanchez,§,∥ Rudy J. M. Konings,† Roberto Caciuﬀo,† and Anthony K. Cheetham‡ †
European Commission, Joint Research Centre, Institute for Transuranium Elements, P.O. Box 2340, D-76125 Karlsruhe, Germany Department of Materials Science and Metallurgy, University of Cambridge, 27 Charles Babbage Road, Cambridge CB3 0FS, United Kingdom § CEA, INAC-SPSMS, FR-38000 Grenoble, France ∥ Université de Grenoble Alpes, INAC-SPSMS, FR-38000 Grenoble, France ‡
S Supporting Information *
ABSTRACT: The hexavalent and heptavalent sodium neptunate compounds Na4NpO5 and Na5NpO6 have been investigated using X-ray powder diﬀraction, Mössbauer spectroscopy, magnetic susceptibility, and speciﬁc heat measurements. Na4NpO5 has tetragonal symmetry in the space group I4/m, while Na5NpO6 adopts a monoclinic unit cell in the space group C2/m. Both structures have been reﬁned for the ﬁrst time using the Rietveld method. The valence states of neptunium in these two compounds, i.e., Np(VI) and Np(VII), respectively, have been conﬁrmed by the isomer shift values of their Mössbauer spectra. The local structural properties obtained from the X-ray reﬁnements have also been related to the quadrupole coupling constants and asymmetry parameters determined from the Mössbauer studies. The absence of magnetic ordering has been conﬁrmed for Na4NpO5. However, speciﬁc heat measurements at low temperatures have suggested the existence of a Schottky-type anomaly at around 7 K in this Np(VI) phase.
In addition, these ternary compounds containing a [Rn]5fn central ion have also attracted considerable attention because of their interesting electronic and magnetic properties.5−7 For actinide oxide compounds, the crystal-ﬁeld interaction is usually of the same order of magnitude as the spin−orbit coupling interaction and electronic repulsion, 8 which makes the interpretation very complex. As the 5f-orbitals of the actinides have a much greater radial extension than the 4f-orbitals of the lanthanides, which are more core-like, the crystal-ﬁeld interaction cannot be treated as a small perturbation of the electronic energy levels as is done for [Xe]4fn rare earths.8 In the case of [Rn]5f1 and [Rn]5f0 electronic conﬁgurations, however, corresponding to hexavalent and heptavalent neptunium, respectively, the contribution from electronic repulsion is removed, which greatly simpliﬁes the interpretation. In the present work, we report structural reﬁnements for hexavalent Na4NpO5 and heptavalent Na5NpO6 using the Rietveld method, as well as their coeﬃcients of thermal expansion derived from high temperature X-ray diﬀraction measurements. X-ray diﬀraction gives information on the
Figure 1. (A) Comparison between the observed (Yobs, in red) and calculated (Ycalc, in black) X-ray diﬀraction pattern of Na4NpO5. Yobs − Ycalc, in blue, is the diﬀerence between the experimental and calculated intensities. The Bragg reﬂections’ angular positions are marked in green. Measurement at λ = Cu Kα1. (B) The inset shows the crystal structure of Na4NpO5 (Na atoms in yellow, O atoms in red, NpO6 octahedra in gray) showing the chains along c of corner sharing NpO6 octahedra. requires great safety precautions, was done with limited quantities in nitrogen-ﬁlled α-gloveboxes. X-ray Powder Diﬀraction. The samples were characterized at room temperature by X-ray diﬀraction using a Bruker D8 Bragg− Brentano X-ray diﬀractometer mounted inside a glovebox and equipped with a curved Ge monochromator (111), a ceramic copper tube (40 kV, 40 mA), and a LinxEye position sensitive detector. The data were collected by step scanning in the range 10° ≤ 2θ ≤ 120°, with an integration time of about 8 h, a count step of 0.02° (2θ), and a dwell of 5 s/step. Structural analysis was performed by the Rietveld method using the Fullprof2k suite.12 The thermal expansion and stability of the Na4NpO5 and Na5NpO6 phases were also assessed by high temperature X-ray diﬀraction using the same diﬀractometer equipped with an Anton Paar HTK 2000 chamber. Measurements were conducted under helium up to 1273 K. The heating chamber was purged several times before the experiment and ﬁlled to about 600−700 mbar. The temperature, measured with a thermocouple, was previously calibrated using the thermal expansion data of MgO.13 The uncertainty on the temperature is estimated to be 20 K at 1473 K. Mö ssbauer Spectroscopy. The 237Np Mössbauer measurements were carried out in transmission, using an 241Am metal source with a sinusoidal driving mode. The eﬀect was measured with a photon energy of 59.54 keV. The Na4NpO5 and Na5NpO6 powder samples, encapsulated in 3 concentric aluminum containers, were measured in the temperature ranges 4.2−20 and 4.2−50 K, respectively, while the source was kept at a constant temperature of 4.2 K inside a stainless steel cryostat. Magnetic Susceptibility Measurements. Magnetic susceptibility measurements were made using a SQUID magnetometer (Quantum Design MPMS-7) from 3 to 301 K, in a ﬁeld of B = 1 T, on a 19.90(5) mg Na4NpO5 sample encapsulated in Stycast 2850 FT. The contribution of the Stycast was subtracted from the recorded data. Speciﬁc Heat Investigations. Low temperature heat capacity measurements were performed on the Na4NpO5 material using a PPMS (Physical Property Measurement System, Quantum Design) instrument, in the absence of a magnetic ﬁeld in the temperature range
structures, but it cannot provide a deﬁnitive signature of the oxidation state of the neptunium ion in those compounds. 237 Np Mössbauer spectroscopy is a very powerful technique for this purpose, which is used herein to conﬁrm the respective Np(VI) and Np(VII) valence states in Na4NpO5 and Na5NpO6. It also gives a direct insight into the electronic and local structural environment around the Np nucleus, as well as the magnetic ﬁeld acting on it.9 The local environment around the neptunium ion is therefore also discussed in this study with respect to the ﬁtted Mössbauer parameters, i.e., quadrupole coupling constants and asymmetry parameters. Moreover, the absence of magnetic ordering is conﬁrmed for both compositions. Finally, speciﬁc heat measurements of Na4NpO5 are reported, which show a broad Schottky-type anomaly around 7 K. Explanations for this feature are suggested.
Sample Preparation. Na4NpO5 and Na5NpO6 were synthesized by grinding together stoichiometric amounts of neptunium dioxide (237NpO2 from JRC-ITU stocks, provided by ORNL, Oak Ridge National Laboratory) and sodium carbonate (Na2CO3 99.95%, Sigma), and heating the mixtures at 1100 K for 60−70 h under oxygen ﬂow with intermediate regrinding steps. Two diﬀerent batches of Na4NpO5 material were prepared. The former, used for Mössbauer spectroscopy and magnetic susceptibility measurements, contained 1.8 wt % of Na5NpO6 impurity, while the latter, used for speciﬁc heat measurements at low temperatures, showed 0.5 wt % of α-Na2NpO4 impurity. The characterization of the sample’s purity for the speciﬁc heat measurement was reported in detail in another publication,10 and the collected data were corrected for the α-Na2NpO4 contribution. As for the Na5NpO6 material, no secondary phases were detected by Xray diﬀraction. 237 Np decays to 233Pa by α emission with a half-life of 2.14 million years. The 233Pa daughter product is a β− emitter with a very short half-life (27 days) and signiﬁcant γ dose rate [1.335 × 10−4 (mSv/h)/ MBq].11 Therefore, the handling of the neptunium samples, which B
Inorganic Chemistry 2.4−292.2 K, and in a 7, 10, and 14 T magnetic ﬁeld in the temperature range 2.4−20.4 K. The PPMS technique is based on a relaxation method, which was critically assessed by Lashley et al.14 The measurements were carried out on 21.07(5) mg of Na4NpO5 material encapsulated in Stycast 2850 FT, and the heat capacity contribution of the Stycast was subtracted from the recorded data. A more detailed description of the experimental procedure, which is particularly well-adapted to the study of radioactive materials, was given in ref 15. The contributions from the sample platform, wires, and grease were also deduced by a separate measurement of an addenda curve. On the basis of the experience acquired on this instrument with standard materials and other compounds,14,15 the uncertainty was estimated at about 1% in the middle range of acquisition, and reached about 3% at the lowest temperatures and near room temperature.
The structure is made of “reverse” neptunyl type of NpO6 octahedra, with two long Np−O(1) bonds at 2.31(1) Å along the axial c direction, and four short Np−O(2) bonds at 2.05(1) Å in the equatorial ab plane, as shown in Figure 2. By contrast, a (NpO2)2+ neptunyl type of conﬁguration consists of two close oxygen neighbors in the axial direction and four distant ones in the equatorial plane. The NpO6 octahedra in Na4NpO5 exhibit perfect axial symmetry, which is important information for the Mössbauer study. Moreover, they share corners between each other forming parallel and inﬁnite chains in the c direction, with a Np−O(1)−Np angle of 180° (Figure 1B). The intrachain Np−Np distance is 4.62(1) Å, and the interchain Np−Np distance is large (5.81(1) Å). The chains can hence be considered as well-isolated from a magnetic point of view. This particular type of reverse neptunyl conﬁguration is unique among the series of sodium neptunate compositions,4 and unusual among the larger family of alkali metal−actinide ternary oxide phases. It is found in the isotructural Na4UO516 and Li4NpO5 compounds.17 This speciﬁc feature is probably related to the Np−O−Np arrangement in chains. As for the sodium atoms, they are located between the chains, and bind them together. The NaO6 octahedra are rather distorted with Na−O bond lengths covering the range 2.33(1)−2.69(1) Å. Finally, the unit cell volume of Na4NpO5 (262.1 Å3) is slightly smaller than the unit cell volume of the isostructural Na4UO5 compound (264.2 Å3),18 which is consistent with the ionic radii for Np6+ (0.72 Å) and U6+ (0.73 Å) according to Shannon’s tabulated data.19 The present X-ray diﬀraction pattern for Na5NpO6, shown in Figure 3, was reﬁned using monoclinic Li5ReO6, in space group C2/m, as a starting model,20 leading to the cell parameters a = 5.829(3) Å, b = 9.996(3) Å, c = 5.757(3) Å, and β = 110.73(1)°. Reﬁned atomic positions are given in Table 2. Keller et al. ﬁrst reported in 1965 the formation of Na6NpO6 by reaction at 723 K between sodium oxide and neptunium oxide mixed in a (3:1) ratio,2,4 and identiﬁed the compound as isostructural with Li6ReO6, but did not perform Mössbauer spectroscopy to conﬁrm the Np(VI) valence state.21 Reproducing the synthesis conditions of Keller et al.,2 Smith et al. have shown that the compound formed was most probably heptavalent Na5NpO6, rather than hexavalent Na6NpO6.4 The sample prepared in this work with sodium carbonate instead of sodium oxide is a nicely crystalline forest green material, of suﬃcient quality for the determination of the structure.
RESULTS AND DISCUSSION X-ray Powder Diﬀraction. Na4NpO5 was reported to be isostructural with Na4UO5, i.e., tetragonal in the space group I4/m by Smith et al.,4 but the quality of the latter X-ray data was not good enough to perform a Rietveld reﬁnement. A new synthesis route using sodium carbonate instead of sodium oxide led to a more crystalline sample in the present work, allowing the determination of the structure. The X-ray diﬀraction pattern for Na4NpO5 is shown in Figure 1A. The reﬁned cell parameters are a = 7.535(3) Å, c = 4.616(3) Å. The atomic positions are listed in Table 1, and selected bond lengths are given in the Supporting Information. Table 1. Reﬁned Atomic Positions in Na4NpO5a atom
Na Np O1 O2
+1 +6 −2 −2
8h 2a 2b 8h
0.198(1) 0 0 0.259(1)
0.403(1) 0 0 0.083(1)
0 0 0.5 0
0.85(1) 0.25(1) 2.49(1) 1.88(1)
Rwp = 17.7%, Rexp = 4.45%, χ2 = 15.9 (standard deviation = 3σ). 5578 points for pattern. 82 reﬁned parameters. Peak shape η: Pseudo-Voigt axial divergence asymmetry. Background: Linear interpolation between operator-selected points in the pattern. The rather large value of Rwp comes from an asymmetric proﬁle in opposite directions for successive hkl reﬂections, which is particularly pronounced at low angles (as shown in the Supporting Information). This is due to slight heterogeneity within the material which creates constraints. It was not possible to improve the reﬁnement using the reﬂection proﬁle functions of the Fullprof software. a
Figure 2. Sketch of the NpO6 octahedra in Na4NpO5 and Na5NpO6. C
Figure 3. (A) Comparison between the observed (Yobs, in red) and calculated (Ycalc, in black) X-ray diﬀraction pattern of Na5NpO6. Yobs − Ycalc, in blue, is the diﬀerence between the experimental and calculated intensities. The Bragg reﬂections’ angular positions are marked in green. Measurement at λ = Cu Kα1. (B) The inset shows the crystal structure of Na5NpO6 (Na atoms in yellow, O atoms in red, NpO6 octahedra in gray) showing the isolated NpO6 octahedra.
Table 2. Reﬁned Atomic Positions for the Na5NpO6 Phasea atom
Np Na1 Na2 Na3 O1 O2
+7 +1 +1 +1 −2 −2
2a 4g 2d 4h 4i 8j
0 0 0 0.5 0.267(1) 0.271(1)
0 0.664(1) 0.5 0.330(1) 0.5 0.354(1)
0 0 0.5 0.5 0.202(1) 0.784(1)
0.66(1) 0.29(1) 0.29(1) 0.29(1) 1.56(1) 1.56(1)
Table 3. Selected Bond Lengths, R (Å), and Angles for Na5NpO6 Derived from the X-ray Diﬀraction Dataa bond Np−O(1) Np−O(2) Na(1)−O(1) Na(1)−O(2) Na(1)−O(2) Na(2)−O(1) Na(2)−O(2) Na(3)−O(1) Na(3)−O(2) Na(3)−O(2) angle
Rwp = 13.7%, Rexp = 3.95%, χ2 = 12.1 (standard deviation = 3σ). 5578 points for pattern. 84 reﬁned parameters. Peak shape η: Pseudo-Voigt axial divergence asymmetry. Background: Linear interpolation between operator-selected points in the pattern. a
The structure of Na5NpO6, in contrast with that of Na4NpO5, comprises isolated NpO65− octahedra in association with charge-compensating Na+ cations. Selected bond lengths and bond angles are listed in Table 3. The NpO6 octahedra have two axial Np−O(1) bonds at 2.08(1) Å and four equatorial Np−O(2) bonds at 2.07(1) Å, as shown in Figure 2. The axial O(1)−Np−O(1) bond is moreover slightly tilted with respect to the equatorial plane [with an O(1)−Np−O(2) angle of 85.8(1)°]. This feature is of importance for the interpretation of the Mössbauer data as detailed in the next section. As for the NaO6 octahedra, they are rather distorted (with minimum and maximum bond lengths 2.28(1) and 2.69(1) Å, respectively). The unit cell volume of isostructural Na5PuO6 synthesized by a very similar procedure,22 i.e., 312.6 Å3, is slightly smaller than that of Na5NpO6 (313.8 Å3), which is consistent with a smaller ionic radius of Pu7+ compared to that of Np7+. Mössbauer Spectroscopy. The Mössbauer spectra of Na4NpO5 recorded at 4.2 and 20 K are shown in Figure 4. They both consist of a broad line due to an unresolved axial (asymmetry parameter η = 0) quadrupole interaction, whose
Standard deviations are given in parentheses. N is the number of atoms in each coordination shell.
quadrupole coupling constant amounts to |e2qQ| = 10.5(3) mm s−1. The isomer shift is δIS = −53.5(3) mm s−1 with respect to NpAl2. Its value lies in the range −32 > δIS > −62 mm s−1, conﬁrming the Np(VI) charge state in Na4NpO5, corresponding to a [Rn]5f1 electronic conﬁguration, as displayed in the correlation diagram in the Supporting Information. The Np ion in this structure is therefore a Kramers ion with a 2F5/2 ground state manifold and 2F7/2 ﬁrst excited state arising from spin− orbit coupling. The investigated material contains a small impurity, however, which manifests itself in the form of a broad line centered at −61.0 mm s−1, corresponding to an isomer shift of δIS = −74.6(3) mm s−1 versus NpAl2. The latter impurity was identiﬁed as Na5NpO6 from the X-ray diﬀraction pattern (1.8 wt %), and estimated to represent about 7% of the D
Figure 5. Isomer shift versus mean neptunium−ligand (Np−L) distance for selected hexavalent neptunium compounds with coordination numbers (CNs) 6 and 8. The red line is a linear ﬁt of the experimental points. Asterisk indicates that, when not available, the mean (Np−L) distance was approximated with the mean (U−L) distance reported by Jové et al.23 and was corrected for the diﬀerence in ionic radius between Np6+ and U6+ according to Shannon’s tabulated data,19 i.e., 0.01 Å.
Figure 4. Mössbauer spectra of Na4NpO5 recorded at 4.2 and 20 K.
total sample from the relative areas of the two subspectra. There is no change in the spectral shape between 4.2 and 20 K, except for a slight decrease in overall intensity with increasing temperature, which was attributed to the temperature dependence of the Lamb−Mössbauer factor. Thus, we can exclude the occurrence of a magnetic phase transition within the probed temperature range. It is interesting to compare the present ﬁtted Mössbauer parameters with those for Li4NpO5, K2NpO4, and β-Na2NpO4 listed in Table 4. The NpO6 octahedra for all four compounds show axial symmetry so that η = 0. The local symmetry around the neptunium ion in Li4NpO5 is also a reverse neptunyl type of conﬁguration, and both compounds, Na4NpO5 and Li4NpO5, have similar values of the quadrupole coupling constant |e2qQ|, 10.5 and 18 mm s−1, respectively, which originates from the slight axial elongation of the NpO6 octahedra. By contrast, K2NpO4 and β-Na2NpO4, which both contain the (NpO2)2+ neptunyl type of ions, have quadrupole coupling constant values around 100 mm s−1. Jové et al., who have investigated correlations among the isomer shift, electric ﬁeld gradient, and local neptunium structure in crystallized and amorphous neptunium compounds covering the Np(III) to Np(VII) valence states,23,24 have pointed out the existence of a linear relationship between the average neptunium−ligand distance and isomer shift for hexavalent neptunium compounds.23,24 The values reported herein for Na4NpO5 ﬁt very well with this trend, as shown in Figure 5. The Np−O mean values of Li4NpO5,17 K2NpO4,22 βNa2NpO4,4,26 and Ba2CoNpO628,29 have been updated in this ﬁgure compared to the values in the ﬁgure of Jové et al.24 The authors also have emphasized a correlation between the values
of the quadrupole coupling constant |e2qQ| and isomer shift, with a separate region for the non-neptunyl compounds NpF6, Ba2CoNpO6, Ba2CuNpO6, and Li4NpO5.24 The Mössbauer parameters found herein for Na4NpO5 satisfy the criteria for this group of compounds, i.e., 0 < |e2qQ| < 50 mm s−1 and −63 < δIS < −52 mm s−1. As for Na5NpO6, the Mössbauer spectra recorded at 4.2, 30, and 50 K, and shown in Figure 6, consist of a single quadrupolar split pattern centered at −61.2 mm s−1, which corresponds to an isomer shift of δIS = −74.8(3) mm s−1 relative to the standard NpAl2 absorber. This shift conﬁrms the Np(VII) valence state. Np(VII) is indeed found in an isomer shift range −60 < δIS < −78 mm s−1 according to the correlation diagram in the Supporting Information. Its value is signiﬁcantly less negative than the free ion Np7+ value estimated to be −194 mm s−1/NpAl2.6 This reveals large partial occupation of the bonding orbitals by the 5f and 6d electrons.30 The measured data were ﬁtted using a quadrupole coupling constant |e2qQ| of 25.9(3) mm s−1, and an asymmetry parameter η (aﬀecting the external line positions) of 0.43(3). A slight decrease in overall intensity was observed with increasing temperature, as expected from the temperature dependence of the Lamb−Mössbauer factor. The Mössbauer parameters found herein are compared in Table 5 to the values reported in the literature for Na5NpO6
Table 4. Structural and Mössbauer Parameters for Some Alkali Oxo-Neptunates compd Na4NpO5 Li4NpO5 K2NpO4 β-Na2NpO4
was related to the increasing occupation of the 5f and 6d atomic orbitals. The parameters reported by Jové et al. for Ba2NaNpO6 and K3NpO5,24 and those found herein for the Na5NpO6 compound, ﬁt this trend very well as shown in Figure 7.
Figure 6. Mössbauer spectra of Na5NpO6 recorded at 4.2, 30, and 50 K.
Table 5. Mössbauer Parameters for Some Alkali Heptavalent Neptunates
δIS (mm s−1/NpAl2)
|e2qQ| (mm s−1)
Na5NpO6 Na5NpO6 Li5NpO6 Li5NpO6 Li5NpO6
−74.8(3) −75.7b −78(2)b −74.8(29)b −77.2(3)b
25.9(3) 24 34(1) 32.9(8) 35(1)
0.43(3) 1 0.34(3) 0.33(1) 0.30(5)
a 24 35 36 30
Figure 7. Variation of the isomer shift with respect to the quadrupole interaction for heptavalent neptunates. The red line is a linear ﬁt of the experimental points.
Magnetic Susceptibility Studies of Na4NpO5. The magnetic susceptibility χM(T) data of Na4NpO5 exhibits paramagnetic behavior from room temperature down to 3 K (Figure 8): No anomaly is observed, conﬁrming the absence of
Present work. bIS value at 4.2 K.
and Li5NpO6. Jov et al. mentioned Mössbauer parameters for Na5NpO6,24 but the corresponding spectrum was, to the authors’ knowledge, never published.31 The isomer shift and quadrupole coupling constant reported, i.e., δIS = −75.7 mm s−1 and |e2qQ| = 24 mm s−1, are very similar to ours, but the asymmetry parameter given by them, η = 1, would correspond to a spectrum with three lines only. This does not correspond to our experimental observation of a quintet. The structure of Li5NpO6 is still a subject of controversy.17,32−34 The most recent study by Morss et al., who performed neutron diﬀraction studies on this compound,17 points toward the monoclinic C2/ m model of Li5ReO6, but a set of six weak reﬂections remains unidentiﬁed. The three sets of Mössbauer parameters reported for Li5NpO6 are nevertheless in good agreement as shown in Table 5. In both cases, i.e., Na5NpO6 and Li5NpO6, the existence of a quadrupole coupling constant |e2qQ|, and nonvanishing asymmetry parameter η, indicates a symmetry lower than Oh. Our X-ray reﬁnement indicates that the O(1)−Np−O(1) axis is tilted by 4° with respect to the equatorial plane (with an O(1)−Np−O(2) angle of 86°), which could explain the presence of an asymmetry parameter. The observed quadrupolar interaction appears to be essentially due to the occupation of the bonding orbitals.30 A neutron diﬀraction study would be required for a more accurate estimation of the Np−O distances and the exact geometry of the NpO6 octahedra. However, by comparison with the data for Li5NpO6, we can suspect a distortion in Na5NpO6 more pronounced than that in Li5NpO6. Finally, looking at general trends among heptavalent neptunium compounds, Friedt et al. reported an increasing linear variation of the quadrupole coupling constant as a function of isomer shift30,37 through the series of compounds Li5NpO6, Cs3NpO5, Rb3NpO5, CsNpO4, and RbNpO4, which
Figure 8. Magnetic suceptibility of Na4NpO5 (red ●) and inverse susceptibility (black ■) as a function of temperature measured at B = 1 T. The dashed line shows the Curie−Weiss ﬁt on the present data.
a magnetic ordering transition in this temperature range, in agreement with previous studies of Bickel et al.38 and the present Mössbauer results. The inverse susceptibility curve 1/χM(T) is linear and obeys a Curie−Weiss law with C = 6.92(2) × 10−2 emu K mol−1 and θP = −15.6(3) K. Although this compound does not order magnetically, the negative value of the Curie temperature suggests the presence of antiferromagnetic interactions. The eﬀective moment inferred from the ﬁt, μeff = 0.74(4)μB, is signiﬁcantly smaller than the value expected for the free Np6+ ion (2.54 μB in Russell−Saunders coupling using the free-ion Jvalue of the ground 2F5/2 multiplet, gJ = 6/7). This lower value is typical for alkali metal−actinide ternary oxides with a [Rn]5f1 F
Inorganic Chemistry central ion,5 where ligand ﬁeld eﬀects are as important as spin− orbit eﬀects. Speciﬁc Heat Investigation of Na4NpO5. The low temperature heat capacity measurements of Na4NpO5 have revealed the existence of a broad anomaly between 3 and 15 K, which was moreover slightly shifted to lower temperatures when a magnetic ﬁeld was applied, as shown in Figure 9.
experimental results, which increases toward high temperatures using the PPMS technique, and on the other hand to the correction for the Stycast contribution. The electronic entropy contribution could arise from an insulator−metal transition, a magnetic order−disorder transition, or a Schottky-type transition associated with crystal-ﬁeld splitting of the energy levels.39 The present Mössbauer measurements performed below and above the temperature of this anomaly, as well as the magnetic susceptibility measurements, have excluded the possibility of a magnetic ordering transition at this temperature. Furthermore, an insulator−metal transition is ruled out as Na4NpO5 is a lime green insulating material. The speciﬁc heat anomaly must hence be due to a Schottky-type behavior arising from low lying electronic energy levels. Its broad shape also resembles a Schottky-type feature rather than the λ peak associated with magnetic ordering. The numerical integration of the (Cp,electronic/T) = f(T) curve in the temperature range 0−35 K using the OriginLab software yielded Selectronic(Na4NpO5, 298.15 K) = 4.57 J K−1 mol−1, i.e., about 79% of the expected order−disorder entropy for such a Kramers system (R ln 2). The electronic levels associated with the 2F5/2 ground state were simulated using a homemade Fortran code in an attempt to reproduce the experimental results. The 2F5/2 ground state has a degeneracy of (2J + 1) = 6, and is therefore split into three Kramers doublets (Γ7 ground state, and Γt7, Γt6 excited states) by the crystal-ﬁeld eﬀect in the tetragonally distorted (D4h) symmetry,5 as shown in the splitting scheme in Figure 11. The 2F7/2 excited state is split in four Kramers doublets.
Figure 9. Evolution of the speciﬁc heat of Na4NpO5 with magnetic ﬁeld.
The excess electronic contribution to the heat capacity was derived hereafter in an attempt to obtain better insight into the origin of the anomaly. The lattice contribution to the heat capacity of Na4NpO5 was approximated with that of the isostructural compound Na4UO5, with the electronic conﬁguration [Rn]5f0, reported in another publication.10 The excess electronic heat capacity obtained from the diﬀerence between these two data is shown in Figure 10. Above 35 K, this electronic heat capacity becomes slightly negative, but this is insigniﬁcant considering the accuracy of the measurement. The heat capacity curves of Na4UO5 and Na4NpO5 cross around 60 K as can be seen in Figure 12, although we would expect the same lattice contribution for both compounds. This discrepancy can be related on the one hand to the uncertainty for our
Figure 11. Splitting of the 5f1 electronic state by (a) spin−orbit coupling, (b) an Oh symmetry, and (c) a D4h symmetry crystal ﬁeld.38
Figure 10 compares the experimental electronic heat capacity with the one calculated for two low lying states having the same degree of electronic degeneracy and separated by 14 cm−1. In Figure 12, the heat capacity of Na4NpO5 is moreover compared with the sum of the lattice contribution of Na4UO5 and excess electronic entropy calculated with the Fortran code. The agreement is rather good, which makes quite a strong case for the existence of a Schottky-type feature. Two conﬁgurations can be envisaged which reproduce these results: one where the Γ7 ground state doublet is split itself by 14 cm−1, the other one where the Γt7 or Γt6 doublet is found 14 cm−1 above the Γ7 ground state doublet. The splitting of the lowest electronic doublet by long-range magnetic ordering was already excluded on the basis of the susceptibility and Mössbauer data. Another explanation for a Γ7
Figure 10. Electronic contribution to the heat capacity in Na4NpO5 obtained by subtracting the data of Na4UO510 (black ●), and comparison with the simulation for energy levels at 0, 14, 5910 cm−1 (blue ●) using a homemade Fortran code. G
110.73(1)°. The ﬁtted Mössbauer parameters, i.e., quadrupole coupling constants and asymmetry parameters, have been related to the local structural properties around the neptunium ion, as inferred from the X-ray reﬁnements. The Np(VI) and Np(VII) valence states in Na4NpO5 and Na5NpO6 have moreover been conﬁrmed by the values of the isomer shifts obtained by Mössbauer spectroscopy, i.e., δIS(Na4NpO5) = −53.5(3) mm s−1/NpAl2 and δIS(Na5NpO6) = −74.8(3) mm s−1/NpAl2. Magnetic susceptibility measurements carried out on Na4NpO5 have conﬁrmed paramagnetic behavior over the entire temperature range, and Curie−Weiss law constants were derived as C = 6.92(2) × 10−2 emu K mol−1 and θP = −15.6(3) K, yielding μeff = 0.74(4) μB for the eﬀective moment. Finally, speciﬁc heat measurements performed on Na4NpO5 at low temperatures have revealed the existence of a Schottky-type anomaly around 7 K. The excess electronic entropy associated with the anomaly was estimated at 4.57 J K−1 mol−1. Simulation using a homemade Fortran code has shown that two low lying electronic states with the same degeneracy and separated by 14 cm−1 could reproduce the experimental results quite well. Our experimental results have brought new insights into the complex electronic structure in this compound, and point to the need for theoretical calculations to elaborate on our results.
Figure 12. Cp/T for Na4UO5 (black ■) and Na4NpO5 (red ●) measured in zero magnetic ﬁeld, and comparison with the sum of the lattice contribution of Na4UO5 and excess electronic entropy obtained by simulating energy levels at 0, 14, 5910 cm−1 (blue ○) using a homemade Fortran code.
ground state splitting would be the occurrence of hyperﬁne interactions with the I = 5/2 nuclear spin of 237Np. Considering that the crystal-ﬁeld potential of the reverse neptunyl geometry is quite close to cubic symmetry, this interaction would split the ground state into two groups (a quintet and a septet) of quasidegenerate levels. However, the magnitude of the splitting required to explain this anomaly would be at least 1 order of magnitude larger than for other Np6+ systems such as NpF6.40 Therefore, the Γ7 doublet should remain degenerate. As for the hypothesis of a Γt7 or Γt6 doublet lying 14 cm−1 above the Γ7 ground state, it would require a complete reevaluation of the spectroscopic data and calculations of Bickel et al.,38,41 according to which the Γ7 ground state is wellisolated.38 Indeed, Bickel et al. performed electronic spectroscopy on Na4NpO5 at 77 K, and reported four bands in the nearinfrared region at 5910, 7225, 8375, and 10 124 cm−1,38 which they assigned to the Γt7 and Γt6 levels, and two nearest doublets of the 2F7/2 levels (Γ′7 and Γt6′). Besides, the latter scenario, which corresponds to a quasiquartet, is not consistent with the observed small value of the eﬀective paramagnetic moment. Therefore, the physical origin of 14 cm−1 splitting remains unclear. Our ﬁndings nevertheless bring new insights into the complex electronic structure of this 5f1 system, and point to the need for theoretical calculations to elaborate on our results. New crystal-ﬁeld investigations would be required to conﬁrm the assignment of Bickel et al. Moreover, the possibility of a splitting of the Γ7 ground state doublet by yet another phenomenon, such as short-range ordering along the magnetic chains, should also be investigated.
S Supporting Information *
X-ray crystallographic ﬁles in CIF format. Selected bond lengths for Na4NpO5. High temperature X-ray diﬀraction studies of Na4NpO5 and Na5NpO6. Correlation diagram for the Mössbauer data. Comments on the magnetic ordering behavior of Li4NpO5. Asymmetric proﬁle shape of Na4NpO5 shown in detail. This material is available free of charge via the Internet at http://pubs.acs.org.
A.L.S. and A.H. contributed equally to this work. Notes
The authors declare no competing ﬁnancial interest.
ACKNOWLEDGMENTS The authors would like to express their gratitude to D. Bouëxière and G. Pagliosa for the collection of room temperature and high temperature X-ray diﬀraction data. A.L.S. acknowledges the European Commission and the Ras al Khaimah Centre for Advanced Materials for funding her Ph.D. studentship.
CONCLUSIONS The present study has used the powerful combination of X-ray diﬀraction and Mössbauer spectroscopy for the investigation of ternary alkali neptunium oxide crystal structures at a very detailed level. The structures of Na4NpO5 and Na5NpO6 have been reﬁned for the ﬁrst time in this work using the Rietveld method. Na4NpO5 crystallizes in the tetragonal system and space group I4/m, with cell parameters a = 7.535(3) Å, c = 4.616(3) Å, while Na5NpO6 adopts monoclinic symmetry, in the space group C2/m, with the following cell parameters: a = 5.829(3) Å, b = 9.996(3) Å, c = 5.757(3) Å, and β =
(1) 2009 GIF R&D Outloook for Generation IV Nuclear Energy Systems; INIS-FR-11-0958; 2009. (2) Keller, C.; Koch, L.; Walter, K. H. J. Inorg. Nucl. Chem. 1965, 27, 1205−1223. (3) Keller, C.; Koch, L.; Walter, K. H. J. Inorg. Nucl. Chem. 1965, 27, 1225−1232. (4) Smith, A. L.; Raison, P. E.; Konings, R. J. M. J. Nucl. Mater. 2011, 413, 114−121. (5) Bickel, M.; Kanellakopulos, B. J. Solid State Chem. 1993, 107, 273−284.
Inorganic Chemistry (6) Kalvius, G. M.; Dunlap, B. D.; Asch, L.; Weigel, F. J. Solid State Chem. 2005, 178, 545−553. (7) Yoshida, Z.; Johnson, S. G.; Kimura, T.; Krsul, J. R. In The Chemistry of the Actinide and Transactinide Elements; Morss, L. R., Edelstein, N., Fuger, J., Katz, J. J., Eds.; Springer: New York, 2006; pp 699−812. (8) Santini, P.; Carretta, S.; Amoretti, G.; Caciuffo, R.; Magnani, N.; Lander, G. H. Rev. Mod. Phys. 2009, 81, 807−864. (9) Dickson, D. P. E.; Berry, F. J. Mössbauer Spectroscopy; Cambridge University Press: New York, 2005. (10) Smith, A. L.; Colineau, E.; Griveau, J.-C.; Raison, P.; Konings, R. J. M. J. Chem. Thermodyn. 2015, submitted. (11) Unger, L. M.; Trubey, D. K. Speciﬁc Gamma-Ray Dose Constants for Nuclides Important to Dosimetry and Radiological Assessment; ORNL/RSIC-45/RI, 1982 (12) Rodriguez-Carvajal, J. Physica B 1993, 192, 55−69. (13) Taylor, D. Br. Ceram. Trans. J. 1984, 83, 5−9. (14) Lashley, J. C.; et al. Cryogenics 2003, 43, 369−378. (15) Javorský, P.; Wastin, F.; Colineau, E.; Rebizant, J.; Boulet, P.; Stewart, G. J. Nucl. Mater. 2005, 344, 50−55. (16) Roof, I. P.; Smith, M. D.; zur Loye, H.-C. J. Cryst. Growth 2010, 312, 1240−1243. (17) Morss, L.; Appelman, E.; Gerz, R.; Martin-Rovet, D. J. Alloys Compd. 1994, 203, 289−295. (18) Smith, A. L.; Raison, P. E.; Martel, L.; Charpentier, T.; Farnan, I.; Prieur, D.; Hennig, C.; Scheinost, A.; Konings, R. J. M.; Cheetham, A. K. Inorg. Chem. 2014, 53, 375−382. (19) Shannon, R. D. Acta Crystallogr., Sect. A 1976, 32, 751−767. (20) Morss, L. R.; Appelman, E. H.; Gerz, R. R.; Martin-Rovet, D. J. Alloys Compd. 1994, 203, 289−295. (21) Keller, C. In Inorganic Chemistry, ser. 1. 7; Bagnall, K., Ed.; Butterworths: London, 1972, p479. (22) Smith, A. L. Unpublished results, 2015 (23) Jové, J.; Cousson, A.; Abazli, H.; Tabuteau, A.; Thévenin, T.; Pagès, M. Hyperfine Interact. 1988, 39, 1−16. (24) Jové, J.; Proust, J.; Pagès, M.; Pyykkö, P. J. Alloys Compd. 1991, 177, 285−310. (25) Nectoux, F.; Jové, J.; Cousson, A.; Pagès, M.; Gal, J. J. Magn. Magn. Mater. 1981, 24, L113−L116. (26) Cordfunke, E. H. P.; IJdo, D. J. W. J. Solid State Chem. 1995, 115, 299−304. (27) Jové, J.; Cousson, A.; Gasperin, M. Hyperfine Interact. 1986, 28, 853−856. (28) Hinatsu, Y.; Doi, Y. J. Solid State Chem. 2006, 179, 2079−2085. (29) Tabuteau, A.; Pagès, M. In Handbook on the Physics and Chemistry of the Actinides; Freeman, A. J., Lander, G. H., Eds.; Elsevier: New York, 1985; Vol. 3, Chapter 4, p 185. (30) Friedt, J. M.; Shenoy, G. K.; Pagès, M. J. Phys. Chem. Solids 1978, 39, 1313−1316. (31) He, L.; Jové, J.; Proust, J.; Pagès, M. 237Np Mössbauer Spectroscopy of Some Ionic Hepta and Hexavalent Oxoneptunates; 19ème Journées des Actinides, Madonna di Campiglio, Italy, 1989; p 11. (32) Scholder, R. Angew. Chem. 1958, 70, 583−614. (33) Wolf, R.; Hoppe, R. Z. Anorg. Allg. Chem. 1985, 528, 129. (34) Hauck, J. Z. Naturforsch. Teil B. 1968, 23, 1603−1603. (35) Bickel, M.; Kanellakopulos, B.; Appel, H.; Haffner, H.; Geggus, S. J. Less-Common Met. 1986, 121, 291−299. (36) Fröhlich, K.; Gütlich, P.; Keller, C. J. Chem. Soc., Dalton Trans. 1972, 971−974. (37) Friedt, J. M. Radiochim. Acta 1983, 32, 105−127. (38) Bickel, M.; Kanellakopulos, B.; Powietzka, B. J. Less-Common Met. 1991, 170, 161−169. (39) Swalin, R. A. Thermodynamics of Solids, 1st ed.; John Wiley & Sons: New York, 1962. (40) Dunlap, B. D.; Kalvius, G. M. In Handbook on the Physics and Chemistry of the Actinides, Vol. 2; Freeman, A. J., Lander, G. H., Eds.; Elsevier: Amsterdam, 1985; pp 71−86.
(41) Kanellakopulos, B.; Keller, C.; Klenze, R.; Stollenwerk, A. H. Physica B. 1980, 102, 221−225.